**“Phase Transformation in Materials”**

**“Phase Transformation in Materials”**

**Eun Soo Park**

**Office: 33-313 **

**Telephone: 880-7221** **Email: espark@snu.ac.kr**

**Office hours: by an appointment**

**2021 Fall**

**10.13.2021**

1

2

**Contents for today’s class **

**• Tracer Diffusion in Binary Alloys**

**• High-Diffusivity Paths**

**1. Diffusion along Grain Boundaries and Free Surface**

**2. Diffusion Along Dislocation**

**• Diffusion in Multiphase Binary Systems**

**D***_{Au}**gives the rate at which Au* (or Au) atoms diffuse in a chemically **
**homogeneous** **alloy, whereas D**_{Au}**gives the diffusion rate of Au when **
**concentration gradient** **is present.**

s b l

### D > D > D

**Grain boundary diffusion makes a significant contribution**

**only when D**_{b}**δ > D****l****d.** **(T < 0.75~0.8 T**_{m}**)**

**At low temperatures, **

**gD**_{p}**/D**_{l}**can become so large** that the apparent diffusivity is entirely
due to diffusion along dislocation.

**(T < ~0.5 T**_{m}**)**

*D* *d* *D*

*D*

_{app}_{=}

_{l}_{+}

_{b}### δ

*S*
*b*

*l*

*A* *A*

*A* > >

**• Atomic Mobility** *D*

_{B}### = *M*

_{B}*RTF* ^{)}

### ln 1 ln

### (

*B*
*B*

*X* *d*

*F* _{=} _{+} *d* γ

**Thermodynamic factor**

} )

( )

( ){ (

1 ^{~} ^{~}

*x*
*D* *C*

*x*
*D* *C*

*C*
*C*

*dt*

*v* *dx* ^{B}^{B}

*B*

*B* ∂

− ∂

∂

∂

= −

= _{β} _{α} α ^{α} β ^{β} **(velocity of the α/β interface)**

### ( )

*B* *A* *A* *B* *B* *A* *A* *B*

*D* = *X D* + *X D* = *F X D*^{*} + *X D*^{*}

3

*** Homework 4 : Exercises 2 (pages 111-114)** **until 1**

^{st}**exam**

**1**

^{st}**exam : October 17, 2021 6 pm – 8 pm** **33-1 dong 228, 327, 328, 330, 331 ho **

**Good Luck!!**

4

**Contents in Phase Transformation**

**(Ch1) Thermodynamics and Phase Diagrams**
**(Ch2) Diffusion: Kinetics**

**(Ch3) Crystal Interface and Microstructure**

**(Ch4) Solidification: Liquid → Solid **

**(Ch5) Diffusional Transformations in Solid: Solid → Solid **
**(Ch6) Diffusionless Transformations: Solid → Solid **

**Background**
**to understand**
**phase **

**transformation**

**Representative**
**Phase **

**transformation**

5

**Chapter 3 Crystal Interfaces and Microstructure**

**Contents for today’s class **

**1) Interfacial Free Energy** **2) Solid/Vapor Interfaces**

**3) Boundaries in Single-Phase Solids**

**4) Interphase Interfaces in Solid (α/β)**

**5) Interface migration**

**Q: Types of interface in metallic system?**

**6**

7

**• Types of Interface**

**1. Free surface (solid/vapor interface)**

**2. Grain boundary (** **α/ α interfaces)**

**> same composition, same crystal structure**

**> different orientation**

**3. inter-phase boundary (** **α/β interfaces)**

**> different composition &**

**crystal structure**

solid vapor

β α defect

energy ↑

**Basically three different types of interface are important in metallic system:**

**: “Important role in determining the kinetics **
**of phase transformation/ complex”**

**→ First, consider simple interfaces, (1) and (2) in this chapter**

**: Important in vaporization and **
**condensation transformations**

**: Important in recrystallization, **
**i.e. the transformation of a **

**highly deformed grain structure **
**into new undeformed grains,**
**and following grain coarsening **
**and grain growth**

**Q: ** **Interfacial free energy, ** **γ vs ** **Surface tension, ** **F?**

**8**

9

**3.1. Interfacial free energy**

**Interfacial energy (γ : J/m**

^{2}**)**

**→ Gibbs free energy of a system containing an interface of area A**

**→ G**

_{bulk}**+ G**

_{interface}### → **G = G**

_{0}**+ γ A**

**solid**

**vapor** **(excess free E arising from the fact **
**that some material lies in or close**
**to the interface)**

**Liquid** **Undercooled Liquid** **Solid**

**<Thermodynamic>**

**Solidification: ** **Liquid** **Solid**

**• Interfacial energy** **Δ**T_{N}

**Melting: ** **Liquid** **Solid**

**• Interfacial energy**
*SV*
*LV*

*SL*

### γ γ

### γ + <

**No superheating required! **

**No Δ**T** _{N}**
T

_{m }vapor

**Melting and Crystallization are Thermodynamic Transitions**

11 NANO STRUCTURED MATERIALS LAB.

**T**

**T**

_{m}12

**Interfacial energy (γ ) vs. surface tension (F: a force per unit length)** **1) work done : F dA = dG**

**2) dG = γ dA + A dγ**

**→** **F = ** **γ + A dγ /dA**

**In case of a liq. film, dγ /dA = 0, F = γ** **(N/m = J/m**

^{2}**)** **Ex) liq. : dγ /dA = 0 **

**sol. : dγ** **/dA ≠ 0, but, very small value**

**At near melting temperature dγ /dA = 0 ** **→ F = γ (N/m = J/m**

^{2}**)**

**3.1. Interfacial free energy**

*Why? *

**Maintain a constatnt surface structure by rearrangement**

**Interfacial energy (γ : J/m**

^{2}**)**

**→ Gibbs free energy of a system containing an interface of area A**

**→ G**

_{bulk}**+ G**

_{interface}### → **G = G**

_{0}**+ γ A**

**solid**
**vapor**

Fig. 3.1 A liquid film on a wire frame.

**(high enough atomic mobility)**

**(excess free E arising from the fact **
**that some material lies in or close**
**to the interface)**

**(independent of A)**

**Q: Free surface (solid/vapor interface)?**

**13**

**(a) ** **E**

_{SV}**vs γ ?**

**Extra energy per atom on surface: ****표면 에너지**

**γ**

**γ**

_{SV}**= 0.15 L**

_{S}**/N**

_{a}### J / surface atom

### • The measured γ values for pure metals near the melting temperature

**E**_{SV}**= 3 ε/2 = 0.25 L**_{S}**/N**_{a}

**(∵ surface free E averaged over many surface plane, S effect at high T) **

**(b) Equilibrium shape: Wulff surface **

**: Polyhedron with the largest facets having the lowest interfacial free energy**

14

**3.2 Solid / Vapor Interfaces**

**- Fcc : **

**density of atoms in these planes decreases as (h**

^{2}**+k**

^{2}**+l**

^{2}**) increases**

**# of Broken Bonds per atom at surface?**

**For (111) plane CN=12**

Fig. 3.2 Atomic configurations on the three closest-packed planes in fcc crystals; (111), (200), and (220).

**( notation {200} and {220} plane has been used instead of {100} and {110} because the spacing of**
**equivalent atom planes is than given by a/(h**^{2}**+k**^{2}**+l**^{2}**)**^{1/2}**where a is the lattice parameter.)**

*** Assumption: S/V interface → Hard sphere model/ uncontaminated surface**

**(In real systems surfaces will reduce their free energies by the adsorption of impurities.)**

15

**# of Broken Bonds per atom at surface?** **→ ** **3 per atom**

16

**Bond Strength: ** **ε ** **for each atom :** **ε/2**

**Excess internal energy over that of the atoms in the bulk: ** **3ε/2 ↑**

**# of broken bond at surface : 3 broken bonds** **For (111) plane**

**For (200) plane CN=12 **

**# of Broken Bonds per atom at surface?**

17

**For (200) plane CN=12 **

**# of Broken Bonds per atom at surface?**

**Bond Strength: ** **ε ** **for each atom :** **ε/2**

**Excess internal energy over that of the atoms in the bulk: ** **4ε/2 ** **↑**

**# of broken bond at surface : 4 broken bonds**

**(excess internal energy of 4ε/2 over that of the atoms in the bulk) **

18

**Bond Strength: ** **ε ** **for each atom :** **ε/2**

**Extra energy per atom on surface: ** **3ε/2 **

**# of broken bond at surface : 3 broken bonds** **For (111) plane**

**Energy per atom of a {111} Surface?**

**Heat of Sublimation **

^{(승화)}**in terms of ε?** **→ ** **L**

_{S}**= 12 N**

_{a}**ε/2** **E**

_{SV}**= 3 ε/2 = 0.25 ** **L**

_{S}**/N**

_{a}**E**

_{SV}**vs γ ?**

### γ **interfacial energy = surface free energy ← Gibb’s free energy **

^{(J/m}

^{2}

^{)}**→ ** **γ = G = H – TS**

**= E + PV – TS**

**(if PV is ignored)**

**→ ** **γ = E**

_{sv}**– TS**

_{sv}**(S**

_{sv }**thermal entropy, configurational entropy)**

**→ ∂γ /∂T = - S **

**: surface free energy decreases with increasing T**

**due to increased contribution of entropy**

**0< S < 3 (mJ/m**^{-2}**K**^{-1}**) **

**“Approximated value” due to assumptions, 1) 2**^{nd}**nearest neighbors have been ignored and**
**2) strengths of the remaining bonds in the surface are unchanged from the bulk values.**

**surface>bulk** **Extra configurational entropy due to vacancies**
**(¼ of L**_{s}**/N**_{a}**)**

**(Latent heat of melting + vaporization)** **(1 mole of solid = 12 N**_{a}**)**

**(E**

_{SV}**↑→ γ ↑)**

19

**γ of Sn : 680 mJ/m**^{2 }**(T**_{m}**: 232ºC)**
**γ of Cu : 1720 mJ/m**^{2}**(T**_{m}**: 1083ºC) **

*** Higher **T_{m}**→ stronger bond (large **L_{S}**) → larger surface free energy (****γ**_{SV}**)**

**cf) G.B. energy γ**_{gb}**is about one third of γ**_{sv}

**γ**

**γ**

_{SV}**= 0.15 L**

_{S}**/N**

_{a}### J / surface atom

### • The measured γ values for pure metals near the melting temperature

*sv*
*s*

*m*

*high* *L* *high*

*T*

*high* → → γ

**• Average Surface Free Energies of Selected Metals**

**측정 어려움, near T**^{m}

**E**_{SV}**= 3 ε/2 = 0.25 L**_{S}**/N**_{a}

**(∵ surface free E averaged over many surface plane, S effect at high T) **

*** E**_{SV}**vs γ ?**

20

### Closer surface packing →

**smaller number of broken bond**

**→ lower surface energy**

**A crystal plane at an angle θ to the close-packed plane will contain broken **
**bonds in excess of the close-packed plane due to the atoms at the steps.**

Low index [ex. (111)]

**(cos** **θ/a)(1/a)**

: broken bonds
**from the atoms on the steps**

**(sin|** **θ|/a)(1/a)**

: additional broken bonds
**from the atoms on the steps**

**# of broken bonds will increase through the series {111} {200} {220} →** **γ****SV ****will increase**
**along the same series (if different entropy term is ignored)**

**Surface energy for high or irrational {hkl} index**

**Surface with high {hkl} index**

Fig. 2.2 The ‘broken-bond’ model for surface energy.

21

**Surface energy for high or irrational {hkl} index**

**(cos** **θ/a)(1/a)**

: broken bonds from the atoms on the steps
**(sin|** **θ|/a)(1/a)**

: additional broken bonds from the atoms on the steps
**Attributing ε/2 energy to each broken bond,**

**E-θ plot**

^{E}

^{SV}**= 3 ε/2 = 0.25 L**

**S**

**/N**

**Fig. 3.4 Variation of surface energy as a function of θ**

_{a}• **The close-packed orientation (θ = 0) lies at a cusped minimum in the E plot.**

**• Similar arguments can be applied to any crystal structure**

**for rotations about any axis from any reasonably close-packed plane.**

• **All low-index planes should therefore be located at low-energy cusps.**

**• If γ is plotted versus θ similar cusps are found (γ-θ plot), but as a result of **
**entropy effects** **they are** **less prominent than in the E-θ plot, and for the higher **
**index planes they can even disappear.**

**Q: Free surface (solid/vapor interface)?**

**22**

**(a) ** **E**

_{SV}**vs γ ?**

**Extra energy per atom on surface**

**γ**

**γ**

_{SV}**= 0.15 L**

_{S}**/N**

_{a}### J / surface atom

### • The measured γ values for pure metals near the melting temperature

**E**_{SV}**= 3 ε/2 = 0.25 L****S** **/N**_{a}

**(∵ surface free E averaged over many surface plane, S effect at high T) **

**(b) Equilibrium shape: Wulff surface **

**: Polyhedron with the largest facets having the lowest interfacial free energy**

**Equilibrium shape: Wulff surface**

### * Distance from center : γ

_{sv}

### Several plane A

_{1}

### , A

_{2}

### etc. with energy γ

_{1}

### , γ

_{2}

### Total surface energy : A

_{1}

### γ

_{1 }

### + A

_{2}

### γ

_{2 .}

### …

### = ∑ A

_{i }

### γ

_{i }

### → minimum

### → equilibrium morphology

### How is the equilibrium shape determined?

1
*n*

*i* *j*
*i*

*A* γ *Minimum*

=

## ∑ = _{γ-θ plot}

_{γ-θ plot}

**Wulff plane**

**: can predict the equilibrium shape of **
**an isolated single crystal**

**Due to entropy effects the plot are**
**less prominent than in the E**_{SV}**-θ plot, **
**and for the higher index planes they **
**can even disappear**

### *

**A convenient method for plotting the variation of γ with surface orientation in 3 dimensions**

**→ Construct the surface using**γ_{sv }**value as a distance between the surface and the origin when measured **
**along the normal to the plane**

24

**Process of Wulff shape intersection for two cubic Wulff shapes**

**: Polyhedron with the largest facets having the lowest interfacial free energy**

25

**Equilibrium shape**

**can be determined experimentally by annealing**

**small single crystals at high temperatures in an inert atmosphere, or**

**by annealing small voids inside a crystal.**

**Of course **

**when γ is isotropic**

**, as for liquid droplets, both the γ-**

**plots and equilibrium shapes are**

**spheres**

**.**

**Equilibrium shape: Wulff surface**

**“Equilibrium shape of FCC crystals”**

**Cannot appear {110} **

**plane in FCC crystals** **1) Square faces {100} and**
**2) Hexagonal faces {111}**

**The length OA represents the **
**free energy of a surface **

**plane whose normal lies in **
**the direction OA.**

**A possible (110) section through the ****γ-plot of an fcc crystal**

**Q: Grain boundary (α/ α interfaces)**

**= Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries** **(b) Special High-Angle Grain Boundaries** **(c) Equilibrium in Polycrystalline Materials**

**26**

27

**Grain boundary**

L . .

. .

.

→ . →

(hkl)

**Single phase - Poly grain**

**1) misorientation of the two adjoining grains**

### (hkl)

**G.B.**

**3.3 Boundaries in Single-Phase Solids: definition**

**(α/α interfaces)**

**2) orientation of the boundary plane**

**> same composition, same crystal structure**

**> different orientation**

**두 개 인접한 결정립간 방위차이 cf. 두 조밀면 만남** **인접 결정립과 입계면의 방위관계**

28

**3.3 Boundaries in Single-Phase Solids**

**tilt boundary** **twist boundary**

### θ **→ misorientation**

**→ tilt angle** θ **→ ** **misorientation**

**→ twist angle** **symmetric tilt** **or twist** **boundary**

**non-symmetric tilt or twist** **boundary**

**: The lattices of any two grains can be made to coincide by rotating**
**one of them through a suitable angle about a single axis.**

*** Relatively simple boundary: relative orientation of the crystals and the boundary**

**Axis of rotation: parallel to the plane of the boundary** **Perpendicular to the boundary**

29

**3.3.1 Low-Angle and High-Angle Boundaries**

**Low-Angle Boundaries**

**An array of parallel edge dislocation** **Cross-grid of two sets of screw dislocations**

**Symmetrical low-angle tilt boundary** **Symmetrical low-angle twist boundary**

Fig. 3.7 (a) Low-angle tilt boundary, (b) low-angle twist boundary: ○ atoms in crystal below, ● atoms in crystal above boundary.

30

**tilt Boundaries**

31

**Dislocations**

32

**twist Boundaries**

33

**Screw dislocation**

34

**Growth of Screw dislocation**

35

**If the boundary is unsymmetrical, dislocations with different** **burgers vectors are required to accommodate the misfit.**

**In general boundaries of a mixture of the tilt and twist type, **

**→ several sets of different edges and screw dislocations. **

**Non-symmetric Tilt Boundary **

Fig. 3.8 An unsymmetrical tilt boundary. Dislocations with two different Burgers vectors are present.

**3.3.1 Low-Angle and High-Angle Boundaries**

**Low-Angle Tilt Boundaries**

**→ around edge dislocation : strain ↑**

**but, LATB ~ almost perfect matching**

**→ g.b. energy : γ****g.b.** **→ E /unit area**

**(energy induced from dis.)**

**Angular mis-orientation **
**across the boundary**
**Burgers vector of **
**the dislocations**

**Energy of LATB ~ Total E of the dislocations within unit area of boundary**

**~ depends on the spacing of the dislocations (D) ** ^{36}

(For brevity, the distinction between internal E and free E will usually not be made from now)

37

**→ around edge dislocation : strain ↑**
**but, LATB ~ almost perfect matching**

**→ g.b. energy : γ****g.b.** **→ E /unit area**

**(energy induced from dis.)**

**Sinθ = b/D , at low angle**

**→ D=b/θ → γ****g.b.** **is proportional to 1/D **

**→ Density of edge dislocation in low**
**angle tilt boundary **

**(cf. low angle twist boundary ****→ screw dis.)**

*** Relation between D and γ ?**

**Very small θ → **
**Very large D**

### θ γ ∝ **3.3.1 Low-Angle and High-Angle Boundaries**

**Low-Angle Tilt Boundaries**

**Energy of LATB ~ total energy of the dislocations within unit area of boundary**

**~ depends on the spacing of the dislocation (D)**

38

**1) As θ increases, γ****g.b.** **↑**

ㅗ ㅗ ㅗ

ㅗ ㅗ ㅗ ㅗ ㅗ ㅗ

**Strain field overlap**

**→ cancel out**

**→ 2) γ****g.b.** **increases and the increasing rate of **

### γ

**(=d γ/d θ) decreases.**

**→ 3) **^{if }**θ increases further, it is impossible to physically identify the individual dislocations**

**→ 4) When θ** **> 10°-15°, increasing rate of γ**_{g.b.}**~ 0**

**Low-Angle tilt Boundaries**

**5) When θ** **> 10°-15°,** **Grain-boundary energy ~ almost independent of misorientation**

### θ

### γ ∝

Fig. 3.11 Rafts of soap bubbles showing several grains of varying misorientation. Note that the boundary with the smallest misorientation is made up of a row of dislocations, whereas the high-angle boundaries have a disordered structure in which individual dislocations

cannot be identified. ^{39}

**Soap Bubble Model** **Structural difference between low-angle and high angle grain boundary**

**Fit very well/ very little free volume/ slightly distorted**

**Large area of poor fit/relatively open structure/highly distorted**

40

**High Angle Grain Boundary: ** **θ** **> 10°-15°**

### High angle boundaries contain large areas of poor fit and have a relatively open structure.

### → high energy, high diffusivity, high mobility (

**cf. gb segregation**

### )

**→ Broken Bonds**

Fig. 3.10 Disordered grain boundary structure (schematic).

41

**Low angle boundary**

**→ almost perfect matching (except dislocation part)**
**High angle boundary (almost)**

**→ open structure, large free volume**

*** low and high angle boundary**
**high angle γ**_{g.b.}**≈ 1/3 γ****S/V.**

**High Angle Grain Boundary**

**Measured high-angle grain boundary energies**

**→ Broken Bonds**

*** As for γ**_{S/V}**,** **γ**_{b}**is temperature dependent decreasing somewhat with increasing temperature. **

**Q: Grain boundary (α/ α interfaces)**

**= Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries** **(b) Special High-Angle Grain Boundaries** **(c) Equilibrium in Polycrystalline Materials**

**42**

43

**: high angle boundary but with low γ**_{g.b. .}

**symmetric twin boundary**

**→ low γ**_{g.b. .}

**Coherent twin boundary** **Incoherent twin boundary**

**(b) Special High-Angle Grain Boundaries I**

**asymmetric twin boundary**

**→ low γ**_{g.b. .}

**Atoms in the boundary **
**are essentially in **

**undistorted positions**

**Energy of twin boundary~ **

**very sensitive to the orienta-**
**tion φ of the boundary plane**

**Twin boundary ≠ Twinning plane**

**Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries**

b) a)

44

**Twin boundary**

45

**Twin boundary**

46

**Twin boundary**

47

**c) Twin boundary energy as a function of the grain boundary orientation**

**Table 3.3 Measured Boundary Free Energies for Crystals in Twin Relationships**

**(Units mJ/m**^{2}**)**

### << <

**(b) Special High-Angle Grain Boundaries I**

48

**Why are there cusps in Fig. 3.13 (b)?**

**Two grains ~ a rotation about a (100) axis**

**In FCC metal, several large-angle orientations with significantly lower energies **
**than the random boundaries. **

**φ =70.5° ~ coherent twin boundary ****(next page), others ~ not well understood**
**a rotation about a (110) axis**

**Most high angle GB~ same E**

**<**

Fig. 3.13 Measured grain boundary energies for symmetric tilt boundaries in Al (a) When the rotation axis is parallel to (100), (b) when the rotation axis is parallel to (110).

**(b) Special High-Angle Grain Boundaries II**

49

**• symmetrical tilt boundary **

**~38.2 °**

**• a small group of**
**atoms are repeated**
**regular intervals**
**along the boundary.**

**~relatively little free volume **

Fig. 3. 14 Special grain boundary: two dimensional example.

**입계의 원자구조가 주위의 격자와 폭넓게 잘 일치 됨**

50

**(c) Equilibrium in Polycrystalline Materials**

**2) ** **Thermally Activated Migration of Grain Boundaries**

**-** **Grain coarsening at high T, annealing due to ****metastable equilibrium ****of GB**

**3) ** **Kinetics of Grain Growth**

**- Grain boundary migration by thermally activated atomic jump**
**- Mobility of GB ~ GB structures and GB segregations**

**4) ** **Effect of second-phase particle on GB migration**

**: Zener Pinning**

max

4
3 _{v}*D* *r*

= *f*

**< Boundaries in Single-Phase Solids >**

**GBs in a polycrystal can adjust themselves during annealing **
**to produce a metastable equilibrium at the GB intersections.**

**1)** **GB intersection: Balance of 1) boundary E & 2) surface tension**

**i.e Normal grain growth Abnormal grain growth**

**“Phase Transformation in Materials”**

**“Phase Transformation in Materials”**

**Eun Soo Park**

**Office: 33-313 **

**Telephone: 880-7221** **Email: espark@snu.ac.kr**

**Office hours: by an appointment**

**2021 Fall**

**12**

^{th}**lecture**

1

2

**Chapter 3 Crystal Interfaces and Microstructure**

**1) Interfacial Free Energy** **2) Solid/Vapor Interfaces**

**3) Boundaries in Single-Phase Solids**

**4) Interphase Interfaces in Solid (α/β)**

**5) Interface migration**

**(a) ** **E**

_{SV}**vs γ ?**

**Extra energy per atom on surface: ****표면 에너지**

**γ**

**γ**

_{SV}**= 0.15 L**

_{S}**/N**

_{a}### J / surface atom

### • The measured γ values for pure metals near the melting temperature

**E**_{SV}**= 3 ε/2 = 0.25 L**_{S}**/N**_{a}

**(∵ surface free E averaged over many surface plane, S effect at high T) **

### γ **interfacial energy = surface free energy ← Gibb’s free energy **

^{(J/m}

^{2}

^{)}**→ ** **γ = E**

_{sv}**– TS**

_{sv}**(S**

_{sv }**thermal entropy, configurational entropy**

**)**

**→ ∂γ /∂T = - S **

**: surface free energy decreases with increasing T**

**due to increased contribution of entropy**

**0< S < 3 (mJ/m**^{-2}**K**^{-1}**) **

**“Approximated value” due to assumptions, 1) 2**^{nd}**nearest neighbors have been ignored and**
**2) strengths of the remaining bonds in the surface are unchanged from the bulk values.**

**Surface > Bulk** **Extra configurational entropy due to vacancies**

**(E**

_{SV}**↑→ γ ↑)**

**Contents for previous class**

**1) Interfacial Free Energy**

3

**Interfacial energy (γ : J/m**

^{2}**)**

**→ Gibbs free energy of a system containing an interface of area A**

**→ G**

_{bulk}**+ G**

_{interface}### → **G = G**

_{0}**+ γ A**

**solid**

**vapor** **(excess free E arising from the fact **
**that some material lies in or close**
**to the interface)**

4

**Surface energy for high or irrational {hkl} index**

**(cos** **θ/a)(1/a)**

: broken bonds from the atoms on the steps
**(sin|** **θ|/a)(1/a)**

: additional broken bonds from the atoms on the steps
**Attributing ε/2 energy to each broken bond,**

**E-θ plot**

^{E}

^{SV}**= 3 ε/2 = 0.25 L**

**S**

**/N**

_{a}Fig. 3.4 Variation of surface energy as a function of θ

• **The close-packed orientation (θ = 0) lies at a cusped minimum in the E plot.**

**• Similar arguments can be applied to any crystal structure**

**for rotations about any axis from any reasonably close-packed plane.**

• **All low-index planes should therefore be located at low-energy cusps.**

**• If γ is plotted versus θ similar cusps are found (γ-θ plot), but as a result of **
**entropy effects** **they are** **less prominent than in the E-θ plot, and for the higher **
**index planes they can even disappear.**

**Contents for previous class**

**2) Solid/Vapor Interfaces**

**Equilibrium shape: Wulff surface**

### * Distance from center : γ

_{sv}

### Several plane A

_{1}

### , A

_{2}

### etc. with energy γ

_{1}

### , γ

_{2}

### Total surface energy : A

_{1}

### γ

_{1 }

### + A

_{2}

### γ

_{2 .}

### …

### = ∑ A

_{i }

### γ

_{i }

### → minimum

### → equilibrium morphology

### How is the equilibrium shape determined?

1
*n*

*i* *j*
*i*

*A* γ *Minimum*

=

## ∑ = _{γ-θ plot}

_{γ-θ plot}

**Wulff plane**

**: can predict the equilibrium shape of **
**an isolated single crystal**

**Due to entropy effects the plot are**
**less prominent than in the E**_{SV}**-θ plot, **
**and for the higher index planes they **
**can even disappear**

### *

**A convenient method for plotting the variation of γ with surface orientation in 3 dimensions**

**→ Construct the surface using**γ_{sv }**value as a distance between the surface and the origin when measured **
**along the normal to the plane**

**3) Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries**

**(b) Special High-Angle Grain Boundaries**

**Θ < 15° : total energy of the dislocations within**
**unit area of boundary**

**Θ > 15° :** **impossible to physically identify the **
**individual dislocations → strain field **
**overlap → cancel out**

**high angle γ**_{g.b.}**≈ 1/3 γ****S/V.**

**Broken Bonds** →

**: high angle boundary but with low γ**_{g.b.}

**→ twin boundary**

**Atoms in the boundary are essentially in undistorted **
**positions ~relatively little free volume **

**Contents for previous class**

**Q: Grain boundary (α/ α interfaces)**

**= Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries** **(b) Special High-Angle Grain Boundaries** **(c) Equilibrium in Polycrystalline Materials**

**7**

8

**: high angle boundary but with low γ**_{g.b. .}

**symmetric twin boundary**

**→ low γ**_{g.b. .}

**Coherent twin boundary** **Incoherent twin boundary**

**(b) Special High-Angle Grain Boundaries I**

**asymmetric twin boundary**

**→ low γ**_{g.b. .}

**Atoms in the boundary **
**are essentially in **

**undistorted positions**

**Energy of twin boundary~ **

**very sensitive to the orienta-**
**tion φ of the boundary plane**

**Twin boundary ≠ Twinning plane**

**Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries**

b) a)

9

**Twin boundary**

10

**Twin boundary**

11

**Twin boundary**

12

**c) Twin boundary energy as a function of the grain boundary orientation**

**Table 3.3 Measured Boundary Free Energies for Crystals in Twin Relationships**

**(Units mJ/m**^{2}**)**

### << <

**(b) Special High-Angle Grain Boundaries I**

13

**Why are there cusps in Fig. 3.13 (b)?**

**Two grains ~ a rotation about a (100) axis**

**In FCC metal, several large-angle orientations with significantly lower energies **
**than the random boundaries. **

**φ =70.5° ~ coherent twin boundary ****(next page), others ~ not well understood**
**a rotation about a (110) axis**

**Most high angle GB~ same E**

**<**

Fig. 3.13 Measured grain boundary energies for symmetric tilt boundaries in Al (a) When the rotation axis is parallel to (100), (b) when the rotation axis is parallel to (110).

**(b) Special High-Angle Grain Boundaries II**

14

**• symmetrical tilt boundary **

**~38.2 °**

**• a small group of**
**atoms are repeated**
**regular intervals**
**along the boundary.**

**~relatively little free volume **

Fig. 3. 14 Special grain boundary: two dimensional example.

**입계의 원자구조가 주위의 격자와 폭넓게 잘 일치 됨**

15

**Contents for today’s class **

**(c) Equilibrium in Polycrystalline Materials**

**②** **Thermally Activated Migration of Grain Boundaries**

**-** **Grain coarsening at high T, annealing due to ****metastable equilibrium ****of GB**

**③** **Kinetics of Grain Growth**

**- Grain boundary migration by thermally activated atomic jump**
**- Mobility of GB ~ GB structures and GB segregations**

**④** **Effect of second-phase particle on GB migration**

**: Zener Pinning**

max

4
3 _{v}*D* *r*

= *f*

**< Boundaries in Single-Phase Solids >**

**GBs in a polycrystal can adjust themselves during annealing **
**to produce a metastable equilibrium at the GB intersections.**

**①** **GB intersection: Balance of 1) boundary E & 2) surface tension**

**i.e Normal grain growth Abnormal grain growth**

**Q: Grain boundary (α/ α interfaces)**

**= Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries** **(b) Special High-Angle Grain Boundaries** **(c) Equilibrium in Polycrystalline Materials**

**16**

**① GB intersection: Balance of 1) boundary E & 2) surface tension**

**GBs in a polycrystal can adjust themselves during annealing **
**to produce “a metastable equilibrium at the GB intersections”.**

17

**(c) Equilibrium in Polycrystalline Materials**

**Microstructure → determined by how the different GBs join together in space**
**Examine how the possibility of different GB energies affects the microstructure **
**of a poly crystalline material**

Fig. 3.15 Microstructure of an annealed crystal of austenitic stainless steel.

: contains high-/low-angle GBs as well as (in-)coherent twin Bs with different GB energies

**1) Why GBs exist at all in annealed **
**materials?**

**Equilibrium ~ Mater. with no GB**

∵**G.B.=high-E regions → G ↑**

: never a true equilibrium structure

**→ ****GBs in a polycrystal can adjust **
**themselves during annealing to **

**produce a metastable equilibrium **
**at the GB intersections.**

**2) Conditions for equilibrium at a GB junction**

**by considering the forces that each B exerts on the junction**

θ
γ
*d*
*d*

**Two grains: a plane ****(GB)****, three grains: a line ****(grain edge)****, four grains: at a point ****(grain corner)**

**Poly grain material: consider the factors that control the grain shapes! **

**1)** **F**_{x}**= γ**
**2) F**_{y}**? **

**P is moved at a small distance (δ****y****)**

**A. work done by : ****F**_{y }**δ**_{y}

**B. increase boundary energy caused **

**by the change in orientation δθ ~ l (dγ/dθ) δθ**

**F**_{y }**δ**_{y}**= l (dγ/dθ) δθ**

**→ ****F**_{y }**= dγ/dθ** **torque force** **GB E, γ dependent on θ**
**Forces, **F_{x}**& **F_{y}**, acting at O and P **
**to maintain the B in equilibrium**
**(Eq. 3.3)**

**stationary** **Moving**

**Unit width**

**(∵δ**_{y}**~ l dθ)**

19

(3) (2)

(3) (1) (2)

**F**_{y }**= dγ/dθ**

**→ There is little effect of orientation**

**How metastable equilibrium? → force (torque)**

(1)

**Minimum γ ~ torque = 0 No rotation!**

**입계 E가 입계 방위에 의존한다면, 회전하지 않고**
**유지하기 위해 입계에 cusp까지 끌어당기는 힘에**
**대응하는 힘 작용**

**If Pulling force, F**_{y}**> (dγ/dθ)**_{cusp}**→ Rotating**
**If the GB E is dependent on the orientation **
**of the B, a force dγ/dθ (>0) must be applied **
**to the ends of the boundary** **to prevent it **
**rotating into a lower energy orientation.**

**F**_{y }**= dγ/dθ ~ torque > 0**

**torque = 0**

20

### * General high angle boundary : d γ/dθ ≈ 0 (GB behaves like a soap film)

**→ Under these conditions the requirements for metastable equilibrium at junction **
between three grains is that the boundary tensions γ_{13}, γ_{23}, γ_{12 }must balance.

**→ θ = 120º**

**Ex) If the solid-vapor energy (****γ****S/V****) is **
**the same for both grains,**

**Eq. 3.13 applies to any three boundaries**
**i.e. grain 1~ different phase to grain 2 & 3. **

**grain 2**

**vapor 1**

**grain 3**
If the boundary E is independent of orientation,

**One method of measuring GB energy:**

: anneal a specimen at a high temp. and then measure the angle at the

intersection of the surface with B.

**(Here, presence of any torque terms ~ neglected) **
**The balance of GB tensions for a GB **
**intersection in metastable equilibrium**
**3) **

**(Eq. 3.13) **
**if all GBs have same GB energy independent **
**of boundary orientation **

*** Junction between coherent and incoherent twin boundary segments ** **showing the importance of torque effects**

: the orientation dependence of twin boundary E, Fig. 3.13b

**→ It is energetically favorable for twin boundaries to align themselves**
**parallel to the twinning plane.**

**→ If the boundary is constrained to follow a macroscopic plane that is near but not exactly**
**parallel to the twining plane, the boundary will usually develop ****a stepped appearance**
**with large coherent low-E facets and ****small incoherent high-E risers**.

**→ does not minimize the total twin boundary E but minimize the total free E**

(a) twin boundary in a thin foil specimen as imaged in the TEM

**small incoherent high-E risers**

**large coherent low-E facets **

*** Junction between coherent and incoherent twin boundary segments ** **showing the importance of torque effects**

(a) twin B in a thin foil specimen as imaged in the TEM, (b) & (c), the coherent and incoherent segments of the twin B.

**(b)**

**(c)**
**(a)**

γ_{i }**≤ dγ****c****/dθ**

At the coherent/incoherent twin junction as shown in (b),
incoherent twin B tension, γ**i **must

balanced by a torque term Likewise, coherent twin B tension, γ**c **

must balanced by a torque term

γ_{c}**≥ dγ****i****/dθ**

However, since γ**c**is usually very small,
the incoherent interface need only lie
in a rather shallow energy cusp.

From energy consideration,

if (metastable) equilibrium exists at P in Fig. (c), then a small displacement such as that shown should either produce no change or an increase in the total free energy of the system, i.e. dG > 0

considering unit depth a small displacement δγ at P will increase the total free E by an amount

**dG = l (dγ**_{c}**/dθ) δθ - γ**_{i}**δy > 0** ^{(∵δ}**y** * ~ l dθ)* γ

_{i }**≤ dγ**

_{c}**/dθ**

**Q: Grain boundary (α/ α interfaces)**

**= Boundaries in Single-Phase Solids**

**(a) Low-Angle and High-Angle Boundaries** **(b) Special High-Angle Grain Boundaries** **(c) Equilibrium in Polycrystalline Materials**

**23**

**② Thermally Activated Migration of Grain Boundaries**

**: Grain coarsening at high T, annealing due to ****metastable equilibrium ****of GB**

24

**Considering factors of G.B. growth**

**(a) Pinning particle** **(b) 2**

^{nd}**phases**

**(c) Anisotropic σ, M**

**(d) Impurity (solute) drag** **(e) Strain energy**

**(f) Free surface **

25

**3.3.4. Thermally Activated Migration of Grain Boundaries**

**If the boundary is curved in the shape of cylinder, Fig. 3.20a,**

**it is acted on by a force of magnitude γ/r towards its center of curvature.**

**Therefore, the only way the boundary tension forces** **can balance**
**in three dimensions is if the boundary is planar (r = ∞) or if it is **
**curved with equal radii in opposite directions, Fig. 3.20b and c.**

**Net Force due to Surface Tension**

**Balance **

**in three dimensions**

**GB intersection: Balance of 1) boundary E & 2) surface tension**

**A random grain structure is inherently unstable and, on annealing at high temperatures, the **
**unbalanced forces will cause the boundaries to migrate towards their centers of curvature.**

Fig. 3. 20 (a) A cylindrical boundary with a radius of curvature r is acted on by a force γ/r.

(b) A planar boundary with no net force. (c) A doubly curved boundary with no net force.

**a) Direction of Grain Boundary Migration during Grain Growth**

**For isotropic grain boundary energy in two dimensions, **
**Equilibrium angle at each boundary junction?**

**→ 120**

^{o}**Boundaries** around Grain

### < 6

**; grain shrink, disappear**

**Boundaries** around Grain

### = 6

**; equilibrium**

**Boundaries** around Grain

### > 6

**; grain growth**

**Morphology of metastable equilibrium state **

**called** **grain growth (or grain coarsening)**

**: at high temperature above about 0.5 T**

_{m}**Reduce the # of grains, increase the mean grain size, reducing the total G.B. energy**

**Equilibrium angle at each boundary junction in 3D?**

**→ 109**

^{o}**28’**

**Migration during annealing**
**Effect of different boundary curvatures **

**in two dimensions**

**3 boundaries intersections**
**A corner formed **
**by 4 grains**

Fig. 3. 21 Two-dimensional GB configurations, The arrows indicate the directions boundaries will migrate during grain growth.

27

**Grain Growth (Soap Bubble Model)**

Fig. 3.22 Two-dimensional cells of a soap solution illustration the process of grain growth. Numbers are time in minutes.

28

**Example of Grain Growth simulation in 3D**

Fir. 3. 23 (a) The atomic mechanism of boundary migration. The boundary migrates to the left if the jump rate

from grain 1 → 2 is greater than 2 → 1. Note that the free volume within the boundary has been exaggerated for clarity.

(b) Step-like structure (돌출맥 구조) where close-packed planes protrude into the boundary. 29

**b) Grain Coarsening at High Temp. annealing (above about 0.5 T**_{m}**): **

**The atoms in the shrinking grain detach themselves from the lattice on **
**the high pressure side of the boundary and relocate themselves on a **
**lattice site of the growing grain.**

30

**ΔG = 2γV****m****/r ~ **

**Δμ**

**: effect of pressure difference by curved boundary**

### * Grain coarsening at high T annealing

**→ metastable equilibrium state**
**: # ↓ , size ↑**

High energy Low energy

←

**Driving force for grain growth : F**

**If unit area of GB advances a distance ****δx, # of moles**

**1) Pulling force** **per unit area of boundary :** (

^{-2}### )

*m*

*F* *G* *N m* *V*

### = ∆

**curvature ~ Δ**P ~ Δμ

**Gibbs-Thomson Eq. **

**Free energy difference per unit volume**
Fig. 3.25 A boundary separating grains with different free energies

is subjected to a pulling force F.

**Applies equally to any boundary whose migration causes**
**a decrease in free energy, i.e. during recrystallization,**
**the boundaries btw the new strain-free grains and the **
**original deformed grains **

**of material that enter grain B**

**δx · (1/V****m****)**

**Work : F dx = (2γV**_{m}**/r) (δx/V**_{m}**)**

**→ F = 2γ/r = ΔG/V**_{m}**(by curvature)**

**Grain A** **Grain B**

**(Eq. 3.18) **

**Q: Grain boundary (α/ α interfaces)**

**(a) Low-Angle and High-Angle Boundaries** **(b) Special High-Angle Grain Boundaries** **(c) Equilibrium in Polycrystalline Materials**

**31**

**③ Kinetics of grain growth **

**→** **D = k’t**

^{n }**( Experimental: n << 1/2, ½ at pure metals or high Temp.)**

**- Mobility of GB~ affected by both type of boundaries and GB segregation **
**or 2**^{nd}**phase precipitation **

**i.e Normal grain growth Abnormal grain growth**

32

**2) How fast boundary moves? : Grain Growth Kinetics**

**Grain boundary migration by thermally activated atomic jump**

*** (1) **

**→**

^{(2) : Flux}**(1) atoms in probable site : n**_{1}**Vibration frequency : ν**_{1}

**A**_{2}**: probability of being accommodated in grain (2)**

### → A

_{2 }

### n

_{1 }

### ν

_{1}

### exp(- ΔG

^{a}

### /RT) atom/m

^{2}

*s = J*

_{1→2}

*** (2) →(1) : Flux**

### → A

_{1 }

### n

_{2 }

### ν

_{2}

### exp[-( ΔG

^{a }

### + *ΔG) /RT] = J*

_{2→1}

### When ΔG >0, there will be a net flux from grain 1 to 2.

**(A**_{2 }**n**_{1}**ν**** _{1}**≈

**A**

_{1 }**n**

_{2 }**ν**

_{2}**= Anν)**

### J

_{net }**=** J

_{1→2}**-** J

_{2→1}**= Anν exp(-ΔG**

^{a}**/RT) [1- exp(-ΔG/RT)]**

**(1)** **(2)**

### When ΔG=0, there is no net boundary movement.

**A**

_{2 }**n**

_{1}**ν**

_{1}### ≈ **A**

_{1 }**n**

_{2 }**ν**

_{2}**= Anν**

**(For a high-angle GB,A**** _{1}**≈

**A**

**≈**

_{2}

_{1)}Effect of the driving force on the kinetics of boundary migration

33

• **If the boundary is moving with a velocity ****v****, the above flux must also be equal to **

2 2 1 1

### /

### exp exp

*m*

*a* *a*

*m*
*a*

*or v M* *G V*

*A n v V* *S* *H*

*where M*

*N RT* *R* *RT*

### = ⋅∆

### ∆ − ∆

###

### =

###

###

2

2 1 1

### exp

*a*
*m*

*a* *m*

*A n v V* *G* *G*

*v* *N RT* *RT* *V*

### ∆ ∆

### = −

###

**→ v/( V**

**→ v/( V**

_{m}**/N**

_{a}**)**

**J = v ** ^{•} **c**

**J = v**

^{•}

_{B}

^{(V}**m**

**/N**

_{a}**: atomic volume)**

### J

_{net}**= A**

_{2}**n**

_{1 }**ν**

_{1}**exp(-ΔG**

^{a}**/RT) [ΔG/RT] **

^{(atom/m}

^{2}

^{s)=}

### v **(V**

_{m}**/N**

_{a}**)**

**M : mobility = velocity under unit driving force ~ ** **exp (-1/T)** *v ~ * _{ΔG/V}

**exp (-1/T)**

_{m }

### driving force

**The boundary migration is a thermally activated process.**

**→ F = ΔG/V**_{m}**If ΔG is small [ΔG << RT] ** **Apply Tayler expansion to exp (- ΔG/RT) term**

**Boundary velocity**

**M: mobility of boundary, **

**i.e., the velocity under unit driving force**
**Diffusion flux**

**순표류속도**

exponentially increase with temp

**(입계 이동은 확산처럼 열활성화 과정)**

34

### 1) driving force F = ΔG/V

_{m}

**→ v = M (ΔG/V**

**→ v = M (ΔG/V**

_{m}

### )

M : exponentially increase with temp.

**v : relation to grain coarsening **

**v : relation to grain coarsening**

### Mean grain size (diameter) : D

### Mean radius of curvature of boundary : r if D ∝ r,

D

### Mean velocity : **v = ** αM (ΔG/V

**v =**

_{m}

### )=dD/dt ( ΔG = 2γV

_{m}

### /r)

### = αM(2γ/D) =dD/dt ^{(} ^{α = }

proportional constant ### ~ 1)

**v**

**v**

**(rate of grain growth)**

*~*

**1/D , **

**1/D ,**

**exponentially increase with**

**T**

**T**

*** Kinetic of grain growth**

**Boundary velocity**
**Pulling force**